Scripta Materialia 134 (2017) 61–65 Contents lists available at ScienceDirect Scripta Materialia journal homepage: www.elsevier.com/locate/scriptamat Regular Article A pathway to microstructural reﬁnement through double pulsed gas metal arc welding L.L. Wang a, H.L. Wei b, J.X. Xue a, T. DebRoy b,⁎ a b School of Mechanical and Automotive Engineering, South China University of Technology, Guangzhou 510641, China Department of Materials Science and Engineering, The Pennsylvania State University, University Park, PA 16802, USA a r t i c l e i n f o Article history: Received 15 January 2017 Received in revised form 18 February 2017 Accepted 20 February 2017 Available online xxxx Keywords: Double pulsed welding Modeling Microstructure Grain reﬁning a b s t r a c t In fusion welding, variations of cooling rate and microstructure are commonly achieved by changing heat input. Here we show that the cooling rates can be adjusted and microstructural features could be reﬁned at constant heat input while changing the pulsing parameters. The temporal variations of cooling rates, solidiﬁcation growth rate and weld geometry during both single and double pulsed welding of an aluminum alloy are examined. Furthermore, microstructures of both single and double pulsed gas metal arc welding are presented to demonstrate signiﬁcant microstructural reﬁnement of double pulsed gas metal arc welds for the same heat input. © 2016 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved. Aluminum alloys are joined by friction stir welding or fusion welding depending on applications [1–4]. For the welding of many intricate parts, gas metal arc welding still remains a widely used process of choice . Defect free, structurally sound and reliable welds can be achieved economically by pulsed gas metal arc welding. Single pulsed gas metal arc welding (SP-GMAW) and double pulsed gas metal arc welding (DP-GMAW) are two important fusion welding methods for the joining of aluminum alloys. Achieving a desired microstructure remains an important goal in fusion welding of aluminum alloys. Here we show that the adjustment of pulsing parameters through the use of DP-GMAW provides a means to control the heating and cooling processes and achieves a reﬁned microstructure. The beneﬁts of using DP-GMAW over SP-GMAW include reduced incidence of porosity in the weld metal [6,7], better ability to bridge the gaps in the butting surfaces particularly in large components  and better ability to control the mode of droplet transfer , all of which affect the structure and properties of welds. DP-GMAW is characterized by its special current waveform which provides signiﬁcant process ﬂexibility and control over that can be attained by the conventional SP-GMAW. Fig. 1 schematically illustrates the current waveform and the temporal variations of the transverse and the longitudinal sections of the welds produced by DP-GMAW. The welding current used during DP-GMAW is characterized by its pulsed waveform in two sets of pulsing frequencies. Typically, the high pulsing ⁎ Corresponding author. E-mail address: [email protected] (T. DebRoy). http://dx.doi.org/10.1016/j.scriptamat.2017.02.034 1359-6462/© 2016 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved. frequency is on the order of 100 Hz and the low pulsing frequency is about 1–5 Hz. The high pulsing frequency is designed to achieve controllable droplet transfer to the liquid metal pool. The low pulsing frequency allows control of the heating and cooling processes during DPGMAW . Periodic variations of fusion zone geometry, peak temperature, cooling rate and solidiﬁcation parameters occur during DP-GMAW due to time dependent heat input and these variations signiﬁcantly affect the microstructure of the weld metal. What is necessary and not available in the literature is a rigorous understanding of how and why the bead geometry and microstructure attained by DP-GMAW evolve with time and differ from those produced by SP-GMAW. In this work, the temporal variations of cooling rate, solidiﬁcation growth rate and weld geometry were calculated using a three-dimensional heat transfer and ﬂuid ﬂow model to correlate these parameters with the scale of microstructures in aluminum alloy 6061 for DP-GMAW and SP-GMAW. Bead-on-plate welding experiments were carried out on aluminum alloy AA6061 base metal (200 × 80 × 4 mm3) using ER4043 ﬁller wire. Chemical compositions of alloys AA6061 and ER4043 are presented in Table 1 . Process parameters of SP-GMAW and DP-GMAW are presented in Table 2. Pure argon was coaxially supplied as shielding gas at a ﬂow rate of 18 L/min. After welding, specimens were cut along transverse and longitudinal cross sections of welds. The samples were ground and polished to 0.06 um using colloidal silica, which were subsequently etched using the standard Keller agent with 10 s for metallographic analysis. The secondary dendrite arm spacing was measured in three locations of both SP-GMA and DP-GMA welds. Each location contained more than six secondary dendrites. 62 L.L. Wang et al. / Scripta Materialia 134 (2017) 61–65 Table 2 Welding process parameters for SP-GMAW and DP-GMAW. Fig. 1. Schematic diagram of current waveform and transverse and longitudinal sections of the DP-GMAW weld pool. The temperature and velocity ﬁelds were calculated using a welltested, transient, three-dimensional heat transfer and ﬂuid ﬂow model that solves the equations of conservation of mass, momentum and energy. The metal transfer mode during SP-GMAW and DP-GMAW is droplet transfer with one droplet per high frequency pulse. A volumetric heat source is incorporated in the model to account for the energy transferred by the overheated droplets into the weld pool [12,13]. Details of the governing equations and boundary conditions can be found in our previous papers and are not repeated here [14–18]. The thermophysical properties used in the heat transfer and ﬂuid ﬂow model are presented in Table 3 [19,20]. The pulsing current of SP-GMAW in the model is implemented as constant mean current of 100 A. Such a simpliﬁcation offers enhanced computational efﬁciency without affecting the accuracy of the calculations. The current pulsing frequency of SP-GMAW was 100 Hz and under such high frequency the weld pool behaves similar to the case of constant current welding . The experimentally observed results show that the weld pool geometry is constant during SP-GMAW . The currents during the ﬁrst and the second pulse phases of DPGMAW, 140 A and 60 A, respectively, are implemented in a similar way to that for SP-GMAW. The temperature gradient (G), growth rate (R) and their combined form GR which represents cooling rate are important solidiﬁcation parameters. The parameters G and R are temporally and spatially variable and they can be calculated from the heat transfer and ﬂuid ﬂow calculations. The value R was calculated at the trailing edge of the melt pool on the top surface using the following relation: R¼ Δds Δt ð1Þ Process parameters SP-GMAW DP-GMAW Mean voltage (V) Mean current (A) Welding speed (mm/s) Wire feeding rate (mm/s) Wire diameter (mm) Density of wire (kg/m3) Frequency (Hz) First phase current (A) Second phase current (A) First phase time (s) Second phase time (s) 22.3 100 8 62 1.2 2685 100 – – – – 22.3 100 8 62 1.2 2685 2.5 140 60 0.2 0.2 Fig. 2 (a), (b) and (c) shows the calculated temperature and velocity ﬁelds in the transverse sections of SP-GMAW and DP-GMAW, respectively. In all cases, the liquid metal ﬂows from the center to the periphery of the melt pool near the top surface driven by Marangoni stress due to the spatial gradient of surface tension. In the molten weld pool, the liquid metal circulates with velocities of about 300 mm/s. At these high velocities, heat is transported mainly by convection within the melt pool. In addition, the size of the SP-GMAW weld pool lies between the largest and the smallest sizes of the weld pools formed by DPGMAW for the same heat input. The ﬁnger penetration characteristic of GMA welding is observed in Fig. 2 (a), (b) and (c). Although the mean current is low for both SP-GMAW and DP-GMAW, the peak current reaches 300 A. The ﬁller wire is rapidly melted and a droplet is generated for each pulse when the peak current is applied. The overheated droplets are accelerated by the electromagnetic force and impinge into the weld pool at a high speed. The resulting transport of heat to the interior of the weld pool causes ﬁnger penetration. It can be observed from Fig. 2 (a), (b) and (c) that the calculated results match well with the experimental data. The depths of penetration of DP-GMAW welds vary with time in a periodic manner as shown in Fig. 2 (e), which is consistent with the temporal variation of heat input. This pattern differs signiﬁcantly from the constant penetration depth of SP-GMAW shown in Fig. 2 (d). The maximum and minimum penetration depths are attained after 1.4 s at the end of ﬁrst pulsing phase and 1.6 s at the end of the second pulsing phase, respectively. An important feature of DP-GMAW is that the peak temperature in the melt pool changes periodically whereas it is constant during SP-GMAW as shown in Fig. 3 (a). Another important outcome of the time dependent heat input during DP-GMAW is the periodic shrinkage and expansion of the melt pool. This variation leads to unusual remelting and resolidiﬁcation of the weld metal. It will be shown subsequently that the unusual temporal variations of the melt pool geometry and cooling rate during DP-GMAW result in a unique solidiﬁcation Table 3 Data used for the calculations [19,20]. Variables and unit Value −3 where Δds is the displacement of the trailing edge during a short time interval of Δt. The cooling rate was calculated near the bottom of the weld pool to match the location for microstructure evaluation. Table 1 Chemical compositions of AA6061 and ER4043 (wt%) . Material Mg Si Fe Cu Mn Cr Al AA6061 ER4043 1.02 0.05 0.75 5.60 0.45 0.80 0.25 0.30 0.06 0.05 0.05 – Bal. Bal. Density of liquid metal (kg m ) Viscosity of liquid (kg m−1 s−1) Solidus temperature (K) Liquidus temperature (K) Enthalpy of solid at melting point (J kg−1) Enthalpy of liquid at melting point (J kg−1) Speciﬁc heat of solid (J kg−1 K−1) Speciﬁc heat of liquid (J kg−1 K−1) Thermal conductivity of solid (W m−1 K−1) Thermal conductivity of liquid (W m−1 K−1) Coefﬁcient of thermal expansion (K−1) Temperature coefﬁcient of surface tension (N m−1 K−1) 2400 0.001 855 925 0.596 0.981 980 1160 168 108 2.375 × 10−5 −3.5 × 10−4 L.L. Wang et al. / Scripta Materialia 134 (2017) 61–65 63 Fig. 2. (a) Transverse section of the SP-GMAW weld. (b) Largest transverse section of the DP-GMAW weld. (c) Smallest transverse section of the DP-GMAW weld. (d) Weld penetration depth versus time of the SP-GMAW weld. (e) Weld penetration depth versus time of the DP-GMAW. condition and microstructure that are signiﬁcantly different from those attained by SP-GMAW. The calculated temporal variation of solidiﬁcation growth rate, R, at the trailing edge of the weld pool is shown in Fig. 3 (b). Unlike SPGMAW, R is time dependent for DP-GMAW. It can be observed from Fig. 3 (b) that during the ﬁrst phase of pulsing that lasts from 1.2 to 1.4 s, the solidiﬁcation growth rate R decreases with time from 1.2 to 1.3 s. This is because the melt pool expands from 1.2 to 1.3 s, with its trailing edge moving in a direction opposite to the welding direction. Despite the constant welding speed, the trailing edge comes to a standstill with R decreasing to 0 mm/s at 1.24 s, which means that the expansion speed of the melt pool at its trailing edge is equal to the welding speed. The growth rate is negative between 1.24 and 1.3 s because the expansion speed of the melt pool is higher than the welding speed. A remelting of the previously solidiﬁed weld metal occurs during this time, which is a strikingly different behavior from that in SP-GMAW. On the other hand, R increases from 1.3 to 1.4 s due to the lower expansion speed of the melt pool compared with the welding speed. Solidiﬁcation growth rate at the trailing edge of the weld pool, R, increases rapidly from 1.4 to 1.5 s within the second pulsing phase which spans from 1.4 to 1.6 s. The higher growth rate originates from the signiﬁcant shrinkage of the melt pool during this period. The overall growth rate is the sum of the shrinkage and welding speeds since both displacements are in the same direction. After the maximum shrinkage velocity is reached at 1.5 s, the growth rate decreases from 1.5 to 1.6 s. The mean value of the solidiﬁcation growth rate, R, is 10.8 mm/s for the DP-GMAW welds. This value is greater than the constant R of SP-GMAW which is 8.0 mm/s. Fig. 3 (c) shows the variation of cooling rate with time near the bottom of the weld pool. The mean value of cooling rate for DP-GMAW, 1735 K/s, is signiﬁcantly higher than the 1330 K/s rate for SP-GMAW. The mean value of the cooling rate of DP-GMAW was calculated from the variable data in Fig. 3 (c). The difference in the cooling rates of the two processes affects the scale of microstructures of the welds. Note that the scale of the solidiﬁcation structure is signiﬁcantly affected by the cooling rate. The relation between the secondary dendrite arm spacing (λ2) and cooling rate (GR) is given as [23,24]: λ2 ¼ aðGRÞ−n ð2Þ Where the exponent n lies between 1/3 and 1/2, and a is a constant whose value depends on the alloy system. Eq. (2) indicates that the secondary dendrite arm spacing decreases with increase in cooling rate. The reﬁned solidiﬁcation structure of welds fabricated by DP-GMAW originates from the higher cooling rate. Fig. 4 shows the microstructures from the transverse sections of the welds by SP-GMAW and DP-GMAW. They were taken from the same position within the welds for a meaningful comparison as indicated by the insert. Additionally, the microstructures and cooling rates are evaluated at the same location which is at the bottom of the weld pool. As expected, the microstructures featured an Al-Si eutectic phase distributed within the α-Al matrix . Cellular structures were observed near the fusion line, which developed into columnar dendrites further away from the fusion line. The cell spacings produced by DP-GMAW were signiﬁcantly smaller than that within the microstructure produced by SPGMAW. The measured secondary dendrite arm spacings were 13.4 ± 2.3 μm and 10.2 ± 0.8 μm for SP-GMAW and DP-GMAW, respectively, consistent with ﬁner solidiﬁcation structure in DP-GMAW for identical mean heat input for the two processes. 64 L.L. Wang et al. / Scripta Materialia 134 (2017) 61–65 Fig. 4. Microstructures of 6061 aluminum alloy welds showing a darker Al-Si eutectic phase distributed within the lighter α-Al matrix. (a) SP-GMAW and (b) DP-GMAW. We thank James S. Zuback for his help in preparing the metallographic specimens. One of the authors acknowledges ﬁnancial support for this research from the High-level Leading Talent Introduction Program of GDAS (2016GDASRC-0106); Industry-university-research Program of Guangdong Province and the Ministry of Education (2013B090600098, 2013B090600030); and the SCUT Doctoral Student Short-Term Overseas Visiting Study Funding Project. Appendix A. Supplementary data Supplementary data to this article can be found online at http://dx. doi.org/10.1016/j.scriptamat.2017.02.034. References      Fig. 3. Calculated temporal variations of (a) peak temperature, (b) solidiﬁcation rate and (c) cooling rate. In summary, double and single pulsed gas metal arc welding of aluminum alloy 6061 were studied both experimentally and theoretically. The periodic shrinkage and expansion of the melt pool during double pulsed welding led to an unusual remelting and resolidiﬁcation behavior of the weld metal. Solidiﬁcation rates and cooling rates were significantly higher for the double pulsed gas metal arc welding than those for the single pulsed welding and these differences were responsible for the signiﬁcant reﬁnement of microstructure during double pulsed welding.            U. Donatus, G.E. Thompson, X. Zhou, Scr. Mater. 123 (2016) 126–129. T. DebRoy, H.K.D.H. Bhadeshia, Sci. Technol. Weld. Join. 15 (2010) 266–270. R. Nandan, T. DebRoy, H.K.D.H. Bhadeshia, Prog. Mater. Sci. 53 (2008) 980–1023. A. Elrefaey, Sci. Technol. Weld. Join. 20 (2015) 280–285. P.L. Threadgill, A.J. Leonard, H.R. Shercliff, P.J. Withers, Int. Mater. Rev. 54 (2009) 49–93. C.L.M. da Silva, A. Scotti, J. Mater. Process. Technol. 171 (2006) 366–372. L.L. Wang, G.C. Heng, H. Chen, J.X. Xue, F.L. Lin, W.J. Huang, Int. J. Adv. Manuf. Technol. 86 (2016) 1841–1851. H. Yamamoto, S. Harada, T. Ueyama, S. Ogawa, Weld. Int. 6 (1992) 580–583. A. Liu, X. Tang, F. Lu, Mater. Des. 50 (2013) 149–155. L.L. Wang, L. Jin, W.J. Huang, M. Xu, J.X. Xue, Mater. Manuf. Process. 31 (2016) 2152–2157. D. Bardel, M. Fontaine, T. Chaise, M. Perez, D. Nelias, F. Bourlier, J. Garnier, Acta Mater. 117 (2016) 81–90. C.H. Kim, W. Zhang, T. DebRoy, J. Appl. Phys. 94 (2003) 2667–2679. D.V. Kiran, J. Cheon, N. Arif, H. Chung, S.-J. Na, Int. J. Adv. Manuf. Technol. 86 (2016) 1453–1474. H.L. Wei, J.W. Elmer, T. DebRoy, Acta Mater. 115 (2016) 123–131. H.L. Wei, J.J. Blecher, T.A. Palmer, T. Debroy, Weld. J. 94 (2015) 135S–144S. A. De, T. DebRoy, Weld. J. 84 (2005) 101S–112S. L.L. Wang et al. / Scripta Materialia 134 (2017) 61–65  S. Mishra, T. DebRoy, J. Appl. Phys. 98 (2005), 044902. .  S. Mishra, T.J. Lienert, M.Q. Johnson, T. DebRoy, Acta Mater. 56 (2008) 2133–2146.  H. Zhao, T. Debroy, Metall. Mater. Trans. B Process Metall. Mater. Process. Sci. 32 (2001) 163–172.  F. Miyasaka, Y. Yamane, T. Ohji, Sci. Technol. Weld. Join. 10 (2005) 521–527.      65 J.W. Liu, Z.H. Rao, S.M. Liao, H.L. Tsai, Int. J. Heat Mass Transf. 91 (2015) 990–1000. L.L. Wang, F.G. Lu, H.C. Cui, X.H. Tang, J. Phys. D. Appl. Phys. 47 (2014) 465204. C. Cicutti, R. Boeri, Scr. Mater. 45 (2001) 1455–1460. S.A. David, J.M. Vitek, Int. Mater. Rev. 34 (1989) 213–245. R. Cao, J. Sun, J. Chen, Sci. Technol. Weld. Join. 18 (2013) 425–433.
© Copyright 2021 Paperzz